**EXPERIMENTAL BEHAVIOR AND DESIGN OF **

1
**REINFORCED CONCRETE EXTERIOR BEAM-COLUMN **

2
**JOINTS STRENGTHENED WITH EMBEDDED BARS **

3
4

### Ridwan Rahman

1*_{, Samir Dirar}

2_{, Yaser Jemaa}

3_{, Marios Theofanous}

4_{, and }

5
### Mohammed Elshafie

5 67

1_{ Lecturer in Civil Engineering, Universitas Riau, Pekanbaru, 28293, Indonesia }

8 9

2_{Senior Lecturer in Structural Engineering, University of Birmingham, Edgbaston, }

10

Birmingham, B15 2TT, United Kingdom 11

12

3_{Lecturer in Civil Engineering, Liverpool John Moores University, Liverpool, L3 3AF, }

13

United Kingdom 14

15

4_{Lecturer in Structural Engineering, University of Birmingham, Edgbaston, Birmingham, }

16

B15 2TT, United Kingdom 17

18

5_{Senior Lecturer in Construction Engineering, University of Cambridge, Cambridge, CB2 }

19

1PZ, United Kingdom 20

21

*_{Corresponding author, Email: [email protected] }

22 23

**Abstract **
24

Shear-deficient reinforced concrete (RC) beam-column joints (BCJs) represent one of the 25

main factors behind the seismic damage suffered by existing concrete infrastructure, as well 26

as the associated loss of life. This study presents a novel technique for strengthening shear-27

deficient RC BCJs. The technique involves embedding carbon fiber reinforced polymer 28

(CFRP) or steel bars into epoxy-filled holes drilled within the joint core. Six exterior RC 29

BCJs were constructed and tested under displacement-controlled cyclic loading. Five 30

specimens, of which four were strengthened with embedded bars, were designed with shear-31

deficient joints according to the pre-1980s building codes. The remaining specimen was 32

adequately designed according to ACI 352R-02. The test parameters are the type (steel or 33

CFRP) and number (4 or 8 bars) of embedded bars. The unstrengthened control specimen 34

experienced joint shear failure in the form of cross-diagonal cracks. The strengthened 35

specimens, namely those strengthened with embedded steel bars, exhibited less brittle failure 36

where damage occurred in the beam region at the early stages of loading, suggesting the 37

outset of a beam hinge mechanism. Additionally, the strengthened specimens exhibited 38

enhancements in joint shear strength, ductility, dissipated energy and stiffness of 21%, 6-39

93%, 10-54% and 2-35%, respectively, compared to the control specimen. This paper also 40

presents a mechanics-based design model for RC BCJs strengthened with embedded bars. 41

The proposed model covers all possible failure modes including yielding of the existing steel 42

reinforcement, concrete crushing and debonding of the embedded bars. The accuracy of the 43

proposed model was checked against the test results. The model gave good predictions with 44

an average predicted-to-experimental ratio of 1.05 and a standard deviation of 0.04. 45

46

**Keywords: Analysis; Beam-column joints; Design; Embedded bars; Fiber reinforced **
47

polymer; Reinforced Concrete; Shear strengthening 48

**Introduction **
49

Recent earthquakes have raised concerns about the resilience of existing reinforced concrete 50

(RC) moment-resisting frame structures (Dolce and Goretti, 2015). In such structures, beam-51

column joints (BCJs) play an important role. Without proper design and detailing of the joint 52

shear reinforcement, as the case is with the majority of the existing RC building stock 53

designed according to the pre-1980s design codes (Bedirhanoglu et al., 2010), BCJs can be 54

the most vulnerable elements during an earthquake and can undergo sudden brittle failure 55

known as joint shear. This can lead to devastating effects including loss of life and severe 56

damage to infrastructure costing billions of US dollars (González et al., 2016). 57

58

Conventional techniques for repairing and/or strengthening of shear-deficient RC BCJs 59

include reinforced or prestressed concrete jacketing, concrete masonry unit jacketing or 60

partial masonry infills, steel jacketing and/or addition of external steel plates (Engindeniz et 61

al., 2005). However, these techniques suffer from the difficulty in handling heavy materials 62

during installation and/or the need for scaffolding. Moreover, heavy materials alter the 63

dynamic characteristics of the existing buildings and consequently careful re-analysis of the 64

structure is usually required (Karayannis et al., 2008). Other retrofit systems for shear-65

deficient RC BCJs include post-tensioned rods mounted diagonally across the joint region 66

(Yurdakul et al., 2018), and nickel-titanium shape memory alloy or steel haunches (Pampanin 67

et al., 2006; Sasmal and Nath, 2017) that connect the upper and lower sides of the beam to 68

the top and bottom sides of the column. However, these systems require mechanical 69

anchoring as well as access to the column and beam faces above and/or below the BCJ 70

region. 71

During the past two decades, the use of fiber reinforced polymer (FRP) strengthening 73

techniques has gained interest due to the excellent mechanical and durability properties of the 74

FRP composites (El-Amoury and Ghobarah, 2002; Ghobarah and Said, 2002; Ghobarah and 75

El-Amoury, 2005; Tsonos, 2008). However, experimental results have shown that FRP 76

debonding remains the main drawback preventing the utilization of the high tensile strength 77

of the FRPs (Antonopoulos and Triantafillou, 2003). When un-anchored externally bonded 78

(EB) or near-surface mounted (NSM) FRP systems are used, debonding which is attributable 79

to the low tensile strength of the concrete cover takes place at a stress level of 20-30% of the 80

ultimate tensile strength of the FRPs (Dirar et al., 2013). On the other hand, adequately 81

anchored FRP strengthening systems can eliminate brittle joint shear failure, have better bond 82

performance and reduce joint stiffness degradation. Yet, the application of EB or NSM FRP 83

strengthening systems requires laborious surface preparation as well as protection against 84

vandalism and fire. 85

86

An important advancement in concrete shear strengthening has been the development of the 87

deep embedment (DE) technique (Valerio et al., 2009), also known as the embedded through-88

section (ETS) technique (Chaallal et al., 2011). Unlike EB and NSM FRP shear strengthening 89

systems, the DE/ETS technique relies on embedding additional shear reinforcement, in the 90

form of steel or FRP bars, within the concrete core. For this purpose, holes are drilled into the 91

concrete core and then injected with an adequate binder to bond embedded bars into the 92

concrete. Experimental and numerical studies on DE/ETS-strengthened RC beams have 93

established the effectiveness of the method (Qin et al., 2015; Qapo et al. 2016) and 94

demonstrated its superiority over externally applied FRP shear strengthening techniques 95

(Chaallal et al., 2011). Nonetheless, to date, there are no detailed studies on the seismic 96

performance of shear-deficient RC BCJs strengthened with embedded bars. 97

98

For the first time, this paper extends the applicability of the DE/ETS technique to RC BCJs 99

with inadequate shear reinforcement. The tests reported in this study assess the effectiveness 100

of the DE/ETS technique at improving the seismic behavior of shear-deficient RC BCJs and 101

examine the effect of number and type (steel vs. FRP) of embedded bars. Furthermore, the 102

paper presents a mechanics-based model for predicting the shear strength of RC BCJs 103

strengthened with embedded bars. The experimental results were used to verify the accuracy 104

of the proposed analytical formulation. 105

106

**Research Significance **
107

Recent earthquakes (e.g. Nepal, 2015; Italy, 2016 and Greece/Turkey, 2017) have 108

demonstrated that poor initial design of BCJs is one of the main reasons for the seismic 109

damage suffered by existing RC infrastructure. This paper addresses this concern by 110

providing a novel and practical technique for strengthening shear-deficient RC BCJs. The 111

new strengthening technique overcomes the premature debonding failure mode associated 112

with external shear strengthening techniques. Not only does this paper identify the effect of 113

some important parameters influencing the seismic performance of strengthened RC BCJs, 114

but also it presents an accurate mechanics-based model for predicting the shear strength of
115
DE/ETS-strengthened RC BCJs.
116
117
**Experimental Program **
118
*Specimens *
119

Six exterior RC BCJ specimens were constructed. One of the specimens was adequately 120

designed according to ACI 352R-02 (2002) whilst the remaining five specimens were 121

designed with deficient joint shear reinforcement to represent RC BCJs built according to 122

pre-1980s building codes. All specimens had the same dimensions and steel reinforcement 123

configuration, as shown in Fig. 1. The number of embedded bars was varied in order to 124

examine the effect of joint shear reinforcement ratio. The tested specimens had a three-part 125

designation. The first part, BCJ, stands for beam-column joint. The second part explains 126

whether a specimen was a control (CS) or strengthened (SS) specimen. The last part clarifies 127

whether a specimen was unstrengthened (A), adequately designed (B), strengthened with 128

steel bars (S#) or strengthened with carbon FRP (CFRP) bars (F#), where # refers to the 129

number of embedded bars in joint core. 130

131

All beams were reinforced with 3 16 mm deformed steel bars as top and bottom 132

longitudinal reinforcement. These bars were bent into the joint core and extended for a 133

*distance of 195 mm (~12db where db* is the bar diameter) to represent earlier design practice

134

in developing countries (Garcia et al., 2014). All beams had 8 mm stirrups. The first stirrup 135

was located at a distance of 50 mm from the column face; then the stirrups were spaced at 136

125 mm center-to-center (c/c) for the following 1000 mm of the beam length. End stirrups 137

were spaced at 50 mm c/c (see Fig. 1) to prevent concrete failure under the applied load. 138

139

Four corner and four internal 16 mm deformed steel bars were used as longitudinal 140

reinforcement whereas 8 mm stirrups were used as shear reinforcement for the columns. In 141

the upper and lower parts of a column, the stirrup close to the beam was placed at 50 mm 142

from the beam face (see Fig. 1) and the consecutive stirrups were spaced at 125 mm c/c for 143

the following 750 mm of the column length. End stirrups were spaced at 50 mm c/c at both 144

column ends to provide additional confinement for the concrete at the loading and support 145

points. The adequately designed specimen BCJ-CS-B had five 8 mm stirrups in the joint 146

core whereas all other specimens had one horizontal closed stirrup in the joint core. Details of 147

the BCJ specimens are listed in Table 1. 148

149

*Materials *

150

The test specimens were constructed using normal weight concrete with a target cylinder 151

compressive strength of 30 MPa. The mix proportions of cement: sand: coarse aggregate for 152

all batches were 1.0: 2.5: 3.0 and the water/cement ratio (w/c) was 0.42. The specimens were 153

cast in a horizontal position and were mechanically vibrated to eliminate voids. They were 154

cured for seven days in the formwork and then stored at room temperature (about 15° C). 155

Polyethylene sheets were used to cover the wet burlap to retain moisture. Table 2 gives the 156

*average concrete compressive (fc) and tensile (fct*) strengths on the day of testing. Except for

157

BCJ-SS-S4, all specimens had concrete compressive strength values ranging from 25 MPa to 158

32 MPa. The average and standard deviation values for the concrete compressive strength of 159

these specimens were 29.8 MPa and 2.9 MPa, respectively. This is very close to the target 160

compressive strength value of 30 MPa. 161

162

Two sizes (8 and 16 mm) of grade B500B deformed steel bars were used as longitudinal and 163

*transverse reinforcement or embedded bars. The average values of the yield strength (fy*),

164

*ultimate strength (fu) and elastic modulus (Es*) of the steel bars obtained from three tests on

165

each bar size are given in Table 3. 166

167

CFRP bars, with a nominal diameter of 8 mm and a nominal cross-sectional area of 50.2 168

mm2, were used as embedded shear reinforcement. The CFRP bars had a tensile strength and 169

elastic modulus of 2300 MPa and 130 GPa, respectively, as declared by the manufacturer. 170

The epoxy resin used for bonding the embedded CFRP and steel bars to the concrete had a 171

compressive strength, tensile strength, elastic modulus and bond strength of 82.7 MPa, 43.5 172

MPa, 1493 MPa and 12.4 MPa, respectively, as certified by the manufacturer. 173

174

*Strengthening application *

175

In order to install the embedded bars, holes were made within the joint core by installing 10 176

mm acrylic rods at the required positions within the joint reinforcement cage before casting 177

the concrete (see Fig. 2). The acrylic rods were removed from the concrete one day after 178

casting. Prior to installing the embedded bars, the holes were enlarged using a 12 mm drilling 179

bit and then cleaned by a wire brush and compressed air to remove any cement or aggregate 180

residues. This procedure was also used to ensure that the holes had rough surfaces and 181

consequently allow for better bond performance between the concrete and the embedded 182

bars. The epoxy adhesive was used to fill two thirds of the holes. The bars were then covered 183

with a thin layer of the adhesive and inserted into the holes. Any excess epoxy was removed. 184

Valerio et al. (2009) demonstrated that it was possible to install embedded bars by drilling 185

holes. Cast-in-concrete holes were used in this study for simplicity. Of note is that, in the case 186

of interior BCJ, the presence of built-in edge beams and slabs makes it difficult to insert 187

horizontally embedded bars into the BCJ core. However, it still possible to insert the 188

embedded bars into diagonally drilled holes. 189

190

*Test setup *

191

The test rig comprised two separate frames. One reaction frame was used to resist the axial 192

load applied on the column whereas the other reaction frame was used to resist the cyclic 193

load applied at the beam end. The upper and lower column ends were allowed to rotate in 194

plane but lateral movements of these ends were prevented (See Fig. 3). A constant axial load 195

of 150 kN was applied on the column using a hydraulic jack. This load represents the gravity 196

load that acts on the column from upper floors and corresponds to an axial load ratio of about 197

8%. This value was based on comparable values used by Antonopoulos and Triantafillou 198

(2003) and Pantelides et al. (2002). The reason for using this value was to limit the beneficial 199

effect of axial load on the shear strength of deficient BCJs (Antonopoulos and Triantafillou 200

(2003); Pantelides et al. (2002)). The column load was continuously adjusted in such a way 201

that the axial load acting on the column remained constant. 202

203

The cyclic load was applied at the beam tip using a 500 kN hydraulic actuator with 100 mm 204

stroke. The loading history depicted in Fig. 4 was based on that proposed by ACI T1.1-01 205

(2001). The first drift ratio was selected to be within the linear elastic response range and, 206

except for the final drift ratio associated with failure; any subsequent drift ratio was chosen to 207

be between 125% and 150% of the previous drift ratio (ACI T1.1-01, 2001). The drift ratio is
208
defined as:
209
Drift ratio =
*L*
(1)
210

where * is the vertical displacement of the beam-end and L is the distance from the loading *
211

*point to the column face (L=1300mm). *
212

213

** Experimental Results and Discussion **
214

*Hysteresis response *

215

The hysteresis response of the tested specimens is given in Fig. 5. The load-displacement 216

response of the control specimen (BCJ-CS-A) is presented in Fig. 5(a). There was no 217

significant stiffness degradation up to ±0.75% drift ratio (±9.8 mm). Due to cracking, the 218

specimen stiffness started to deteriorate gradually from ±0.75% (±9.8 mm) to ±3.00% (±39 219

mm) drift ratio, with rapid degradation taking place after ±3.00% (±39 mm) drift ratio. The 220

specimen reached its maximum load carrying capacity (59 kN) at the first cycle of the 3.00% 221

drift ratio loading step and then the load decreased rapidly. 222

223

For BCJ-SS-S4, the load-displacement response in Fig. 5(b) indicates that the specimen 224

remained elastic up to ±0.35% drift ratio (± 4.6 mm), and subsequently maintained a quasi-225

linear cracked stiffness up to ±2.00% drift ratio (±26 mm). The specimen attained its 226

maximum load carrying capacity (70.8 kN) at 3.00% drift ratio (39 mm). Up to 3.00% drift 227

ratio, pinching length was increasing gradually, indicating that the specimen was capable of 228

dissipating energy. A gradual stiffness degradation took place after the specimen reached its 229

maximum load carrying capacity. 230

231

Fig. 5(c) shows that BCJ-SS-F4 had a quasi-linear load-displacement response up to peak 232

load. The maximum load carrying capacity (71.3 kN) was achieved at the first cycle of the 233

3.00% drift ratio (39 mm). The embedded CFRP bars seem to have controlled crack 234

propagation because there was limited stiffness degradation up to the maximum load carrying 235

capacity. From the second cycle of the ±3% drift ratio (±39 mm) until the end of the test, 236

both the load carrying capacity and stiffness significantly deteriorated. 237

238

For BCJ-SS-S8, the load-displacement response (see Fig. 5(d)) shows that there was no 239

significant stiffness degradation up to ±2.00% drift ratio (±26 mm). The specimen attained its 240

maximum load carrying capacity (63.3 kN) at 3.00% drift ratio (39 mm). Further loading 241

beyond 3.00% drift ratio resulted in significant reduction in both the load carrying capacity 242

and stiffness. 243

For BCJ-SS-F8, the load-displacement response (Fig. 5(e)) was quasi-linear, without 245

significant stiffness degradation, up to a drift ratio of ±1.50% (±19.5 mm). The specimen 246

reached its maximum load capacity (68.7 kN) at the first cycle of the 3.00% drift ratio. Upon 247

further loading, both the overall stiffness and load carrying capacity deteriorated with the 248

increase in drift ratio (displacement). 249

250

Comparable to that of the strengthened specimens, the load-displacement response of BCJ-251

CS-B was quasi-linear (see Fig. 5(f)), without significant stiffness degradation, up to a drift 252

ratio of ±1.50% (±19.5 mm). The specimen reached its maximum load carrying capacity 253

(64.5 kN) at the first cycle of the 3.00% drift ratio (39 mm). A limited yield plateau can be 254

seen in the envelope curve at this load level. Starting at ±4.00% drift ratio (±52 mm) until the 255

end of the test, pinching length increased gradually, indicating the capability of the specimen 256

to dissipate energy. Moreover, both stiffness and strength deteriorated gradually as depicted 257

in Fig. 5(f). 258

259

Fig. 5(g) compares the envelope curves of the tested specimens. Compared to the shear-260

deficient control specimen (BCJ-CS-A), the strengthened specimens had higher, or at least 261

comparable, load and/or deformation capacity in both directions. Fig. 5(g) shows that the 262

experimental response of the tested specimens under positive and negative loading was 263

asymmetric. This is attributable to the fact that loading in a given direction can accumulate 264

damage that affects the response in the opposite direction. 265

266

*Damage evolution and failure mode *

267

The typical crack patterns at peak load are illustrated in Fig. 6 while Fig. 7 quantifies the 268

evolution of damage with drift ratio. The damage index (DI) method (Park and Ang, 1985; 269

Park et al.; 1987) together with the corresponding DIs boundaries (Varum, 2003) were used 270

to quantify damage in the test specimens. At a given drift ratio, the strengthened specimens 271

had lower DI values than the control specimen (BCJ-CS-A). The control specimen reached a 272

DI of 1.0 (nominally corresponding to collapse) at a drift ratio slightly higher than 2.00% 273

whereas the strengthened specimens reached the same DI value at a drift ratio of 3.00% to 274

3.60%. The adequately designed specimen (BCJ-CS-B) had the least damage evolution and 275

approached collapse (DI = 1.0) at a drift ratio of about 4.00%. 276

277

The control specimen (BCJ-CS-A) experienced hybrid local damage in the form of shear 278

cracks in the joint and flexural cracks in the beam. The failure mechanism was characterized 279

by shear damage in the form of cross-diagonal cracks. As a result, a wide concrete wedge 280

developed, leading to the spalling of the outer face of the concrete column after a drift ratio 281

of 3.00%, which is typical of joint shear (JS) failure. This can be attributable to the 282

inadequate shear reinforcement in the joint region. Compared to the control specimen, all 283

strengthened specimens exhibited more enhanced behavior. Damage occurred in the beam 284

region at the early stages of loading, suggesting the outset of a beam hinge (BH) mechanism, 285

and then diagonal cracks propagated into the joint after 1.00% drift ratio. Stable hysteresis 286

behavior with high energy dissipation capacity was also maintained until the end of the test 287

(see Figs. 5(a) to 5(f)). 288

289

*Strain response of the embedded bars *

290

Fig. 8 depicts the envelope curves of load versus strain in the embedded bars, with tensile 291

strain assigned a negative sign. Unfortunately, some strain gauges failed during testing and 292

their results were discarded. 293

The embedded bars exhibited two stages of response during loading. In the first stage, the 295

embedded bars were inactive prior to joint cracking and therefore did not contribute to the 296

shear strength. The second stage is marked by the formation of inclined cracks at a load of 297

approximately 20 kN to 35 kN. After the formation of inclined cracks, the shear links 298

developed strain with increasing load until failure. As can be seen in Fig. 8, none of the 299

embedded steel bars attained the yield strain of 0.29%. 300

301

The effect of type of embedded bar on strain response may be inferred by comparing the 302

results of Group B specimens (BCJ-SS-F4 and BCJ-SS-S4). As can be seen in Fig. 8, the 303

embedded CFRP bars were generally more strained than the embedded steel bars. This may 304

be explained by the lower elastic modulus of the CFRP bars (130 GPa) compared with that of 305

the steel bars (199 GPa). Fig. 8 also shows that, regardless of embedded bar type, the strain in 306

the embedded bars of Group C specimens (BCJ-SS-F8 and BCJ-SS-S8) was generally less 307

than that in the embedded bars of Group B specimens (BCJ-SS-F4 and BCJ-SS-S4). This was 308

to be expected as increasing the number of bars from 4 to 8 bars results in a more distributed 309

strain field in the joint panel and consequently less strain in the embedded bars. 310

311

*Strength *

312

The significant contribution of the embedded bars can be seen in Table 4. All strengthened 313

specimens performed better, in terms of joint shear strength and dissipated energy, compared 314

to BCJ-CS-A. This result demonstrates the potential of the strengthening technique. A 315

substantial improvement in the global performance of BCJ-SS-S4 and BCJ-SS-F4 can be 316

seen in the joint shear stress at peak load, which for both specimens increased by 6% and 317

21%, respectively, for the case of upward loading. Further, specimens SS-S8 and BCJ-318

SS-F8 had increases of 7% and 16%, respectively, in the joint shear stress at peak load 319

compared to that of the control specimen (BCJ-CS-A). The strengthened specimens also 320

showed higher joint shear strength than that of the adequately designed specimen BCJ-CS-B. 321

For example, during upward loading, BCJ-SS-F4 and BCJ-SS-F8 had joint shear stress at 322

peak load that was 11% and 7%, respectively, higher than that of BCJ-CS-B. 323

324

Fig. 9 presents the variation of normalized principal tensile stress with joint shear 325

deformation. Compared to the control specimen (BCJ-CS-A), the strengthened specimens 326

had higher cracked joint stiffness during upward (positive) loading. An exception was BCJ-327

SS-S4 which underwent initial joint cracking and achieved its maximum capacity during the 328

downward (negative) loading direction. Moreover, the normalized principal tensile stress of 329

the strengthened specimens at peak load was higher than that of the control specimen. For 330

example, BCJ-SS-F4 had a normalized principal tensile stress at peak load that was 25% 331

higher than that of the control specimen. The corresponding increases for BCJ-SS-S8 and 332

BCJ-SS-F8 were 22% and 18%, respectively. This further demonstrates the potential of the 333

proposed strengthening technique. 334

335

*Ductility *

336

The displacement ductility is defined as *u*/*y*, where *u* is the beam tip displacement at the

337

load step corresponding to 20% reduction in ultimate load and *y* is the yield displacement as

338

defined by the Equivalent Energy Elastic-Plastic curve (Park, 1989). The embedded bars 339

enhance ductility by controlling crack width, thereby delaying the brittle shear failure of the 340

joint panel (Li and Mobasher, 1998). Table 4 shows that the strengthened specimens 341

generally had higher displacement ductility than that of BCJ-CS-A. A 39% (upward 342

direction) and 93% (downward direction) increase in the displacement ductility of BCJ-SS-343

S4 was observed compared to that of BCJ-CS-A. The corresponding increases at upward 344

loading for specimens BCJ-SS-F4 and BCJ-SS-F8 were 6% and 22%, respectively; while the 345

increases at downward loading for specimens BCJ-SS-F4, BCJ-SS-S8 and BCJ-SS-F8 were 346

27%, 20% and 13%, respectively. These results show that, at least for the case of downward 347

loading, the steel-strengthened specimens had higher displacement ductility than that of the 348

CFRP-strengthened specimens. This result can be explained by the fact that steel bars are 349

ductile by nature whereas CFRP bars exhibit liner elastic behavior up to failure. Of note is 350

that no displacement ductility enhancement was observed during upward loading of BCJ-SS-351

S8. Damage accumulation in the joint prevented the increase in the displacement ductility for 352

the case of upward loading of BCJ-SS-S8. The premature damage and limited ductility of 353

BCJ-SS-S8 can be further explained by the relatively low concrete strength (25 MPa) of this 354

specimen. 355

356

Specimen BCJ-CS-B, as expected, had superior displacement ductility compared to those of 357

the strengthened specimens. The joint shear reinforcement of BCJ-CS-B was designed 358

according to ACI 352R-02 (2002) and aimed at satisfying both strength and ductility 359

requirements. The displacement ductility for specimens BCJ-SS-S4, BCJ-SS-F4, BCJ-SS-S8 360

and BCJ-SS-F8 were 24%, 42%, 48% and 33%, respectively, less than that of BCJ-CS-B. 361

362

*Energy dissipation and stiffness degradation *

363

As depicted in Fig. 10, the energy dissipation levels achieved by the strengthened specimens 364

were generally higher than that achieved by the control specimen, especially at drift levels of 365

1.00% or more. For example, the energy absorbed by the strengthened specimens at 4.00% 366

drift ratio was 14947 kN-mm (BCJ-SS-S4), 11433 kN-mm (BCJ-SS-F4), 10616 kN-mm 367

(BCJ-SS-S8), and 11877 kN-mm (BCJ-SS-F8), representing increases of 54%, 18%, 10% 368

and 23%, respectively, over the corresponding value for the control specimen (BCJ-CS-A). 369

The effect of number of embedded bars on energy dissipation capacity may be inferred by 370

comparing the performance of BCJ-SS-F4 and BCJ-SS-F8. As can be seen in Fig. 10, the two 371

specimens had comparable energy dissipation levels up to 3.00% drift ratio. Beyond this load 372

level, BCJ-SS-F8 had higher energy dissipation capacity than that of BCJ-SS-F4 due to the 373

increased number of embedded bars. Moreover, the energy dissipation levels of the 374

strengthened specimens at 4% drift ratio were comparable to, or higher than, that of the 375

adequately designed specimen BCJ-CS-B, except for BCJ-SS-S8. Again, this can be 376

explained by the relatively low concrete strength of BCJ-SS-S8. 377

378

In general, the stiffness degradation of the strengthened specimens was slower than that of 379

BCJ-CS-A but higher than that of BCJ-CS-B. For example, Fig. 11 shows that at 4.00% drift 380

ratio, the normalized peak-to-peak stiffness of SS-S4, SS-F4, SS-S8 and BCJ-381

SS-F8 was 35%, 2%, 19% and 20% higher than that of BCJ-CS-A, respectively. On the other 382

hand, the normalized peak-to-peak stiffness of SS-S4, SS-F4, SS-S8 and BCJ-383

SS-F8 at 4.00% drift ratio was 4%, 28%, 16%, and 15% lower, respectively, than that of the 384

adequately designed specimen BCJ-CS-B. 385

386

The effect of number of embedded bars on normalized stiffness may be inferred by 387

comparing the performance of BCJ-SS-F4 and BCJ-SS-F8. As can be seen in Fig. 11, the two 388

specimens had similar normalized stiffness up to 1.50% drift ratio. Beyond this load level, 389

BCJ-SS-F8 had higher normalized stiffness values due to the increased number of embedded 390

bars which were more effective in controlling crack opening and limiting deflection. The 391

performance of BCJ-SS-S8 and BCJ-SS-F8 suggest that the embedded bar type has limited 392

effect, if any, on normalized stiffness. 393

*Beam fixed-end rotation *

395

Fig. 12 presents the envelope curves of the normalized load versus fixed-end beam rotation 396

for the tested specimens. The control specimen showed limited beam rotation while the 397

specimens strengthened with embedded steel bars showed more enhanced fixed-end beam 398

rotation than the specimens strengthened with embedded CFRP bars. The beam rotation of 399

BCJ-CS-A at maximum load was 0.0066 radians, while the beam rotations of the 400

strengthened specimens at maximum load varied from 0.0074 radians (BCJ-SS-F8) to 0.0092 401

radians (BCJ-SS-S4), representing increases from 12% to 40%. The relatively small beam 402

rotation of the control specimen indicates the absence of a plastic hinge in the beam. The 403

maximum rotations of SS-S4 and SS-S8 were comparable to that of specimen BCJ-404

CS-B, extending to around 0.03 radians at failure. This suggests the onset of a beam hinge 405

mechanism in these specimens. 406

407

**Analytical Model **
408

An analytical model capable of predicting the shear strength of unstrengthened and 409

strengthened RC BCJs with embedded bars was developed. The model is based on those 410

developed by Pantazopoulou and Bonacci (1992) and Antonopoulos and Triantafillou (2002) 411

and covers BCJ response before and after the yielding of the longitudinal and transverse steel 412

reinforcement. Failure is defined as either concrete crushing or debonding of the embedded 413

bars. As shown in Fig. 13, the model idealizes an exterior BCJ as a two-dimensional frame 414

element; where the column width, column height, beam width and beam height are denoted 415

*as wc, hc, wb and hb* respectively.

416 417

*Assumptions *

418

Fig. 14 shows the adopted joint stress equilibrium for joints with embedded bars. Shear 419

stresses are introduced by direct member action and by bond stress-induced forces that 420

develop along the reinforcement within the joint area (i.e. beam reinforcement, column 421

reinforcement and the embedded steel or CFRP bars). To simplify the model formulation, the 422

*shear stress, ν, is assumed to be uniform along the joint boundaries. Additionally, to replicate *
423

real-life conditions before strengthening where the structure is subjected to its self-weight, it 424

*is assumed that a set of initial normal strain in the transverse direction (ε0t*) and initial shear

425

*strain (γ0*) has developed causing a small deformation in the steel bars (Antonopoulos and

426

Triantafillou, 2002). 427

*The maximum and minimum principal strains, ε1 and ε2* respectively, are linked to the strains

428

*in the longitudinal (l) and transverse (t) directions (see Fig. 14), εl and εt* respectively, through

429
Equation (2):
430
*t*
*l*
*l*
*t*
2
2
1
1
2
tan
(2)
431

*where θ is the inclination (from the t-axis) of the maximum principal strain ε1*.

432 433

*By assuming that: (1) the maximum principal stress in the concrete (σ1*) cannot exceed its

434

tensile strength, which is simply taken as zero; and (2) the direction of principal strains and 435

stresses coincide (when the reinforcement has not yielded), the following equations can be
436
written:
437
*t* tan (3)
438
tan
*l* (4)
439

*where σt and σl* are the average compressive stresses in the concrete in the transverse and

440

longitudinal directions, respectively. 441

442

*Finally, with σ1* = 0, the stress invariant condition states give the minimum principal stress in

443
the concrete (σ2):
444
2 *t* *l* (5)
445
446

Equations (2) to (5) were derived and employed in the work of Pantazopoulou and Bonacci 447

(1992). 448

449

*Shear strengthening model *

450

*Based on horizontal force equilibrium (see Fig. 14a), σt* is given by Equation (6):

451

###

###

*b*

*b*

*h*

*Ft*

*Ft*

*t*

*b*

*t*

*s*

*t*

*h*

*w*

*N*

*f*

*f* (6) 452

*where ρs is the existing stirrup ratio, βt* is a factor to account for the bond conditions along the

453

*main beam reinforcement, ρb is the total longitudinal reinforcement ratio in the beam, ft* is the

454

*average stress in the horizontal stirrups (at mid-width of the joint), ρFt* is the steel or CFRP

455

*embedded reinforcement ratio in the transverse direction, fFt* is the average normal stress in

456

*the steel or CFRP embedded bars at mid-width of the joint and Nh* is the axial compressive

457

*force, if any, acting on the beam (usually Nh* may be taken as zero).

458 459

In a similar manner, vertical force equilibrium (see Fig. 14b) dictates that: 460

##

##

*c*

*c*

*v*

*l*

*c*

*l*

*in*

*c*

*l*

*w*

*h*

*N*

*f *

_{,}(7) 461

*where ρc,in is the total longitudinal reinforcement ratio in the column inside the joint core, βl*

462

is a factor to account for the bond conditions along the main column reinforcement at the 463

*boundaries of the joint core, ρc* is the total longitudinal reinforcement ratio in the column at

*the boundaries of the joint core, fl* is the average stress in the longitudinal reinforcement (at

465

*mid-width of the joint) and Nv* is the axial compressive force acting on the column.

466 467

The bond condition between the reinforcement bars and the concrete is defined by the factors 468

*βt and βl*. For a perfect bond condition, the bond factors are taken as zero; while for negligible

469

bond resistance the bond factors are set equal to 1.0. In an actual condition, the magnitudes of 470

the bond factors could be between these two values (Pantazopoulou and Bonacci, 1992). 471

472

Simplifications are made, as follows, to reduce the number of variables in the problem.
473
* _{t}*

**

_{s}**

_{t}*(8a) 474 and 475 *

_{b}**

_{l}

_{c}_{,}

**

_{in}**

_{l}*(8b) 476*

_{c}*where ρt and ρl* are the effective transverse and longitudinal reinforcement ratios,

477

respectively. 478

479

Based on the stress state in the steel reinforcement, four scenarios are considered, namely: a) 480

before the yielding of the transverse and longitudinal reinforcement; b) after the yielding of 481

the transverse reinforcement but before the yielding of the longitudinal reinforcement; c) 482

after the yielding of both the transverse and longitudinal reinforcement and d) after the 483

yielding of the longitudinal reinforcement but before the yielding of the transverse 484

reinforcement. For each scenario, concrete crushing and debonding of the embedded bars are 485

checked as explained in the solution procedure. 486

487

*Step (a) Before the yielding of the transverse and longitudinal reinforcement *

*Equation (2) is rewritten by substituting ε2 by σ2/Ec, where Ec* is the secant elastic modulus of
489
concrete.
490
*t*
*c*
*l*
*c*
*E*
*E*
2
2
2
tan (9)
491

*Next, the minimum principal stress in the concrete (σ2) is written in terms of ν and tan θ *

492
using Equations (3)-(5).
493
_{}
tan
1
tan
tan
tan
2
2 (10)
494

*Subsequently, substituting Equations (3) and (8a) together with ft = Esεt, and fFT = Ef(εt - ε0t*)

495

*(where Es and Ef* are the elastic moduli of steel and FRP, respectively) into Equation (6)

496 yields: 497

##

_{t}E_{s}

_{t}

_{Ft}E_{f}

_{t}

_{Ft}E_{F}_{0}

_{t}##

tan 1_{}

_{}

_{}

_{}

_{}

_{} (11a) 498

*Note that Nh is taken as zero. Similarly, substituting Equations (4) and (8b) together with fl* =

499

*Esεl* into Equation (7) yields:

500

###

_{l}

_{s}

_{l}

_{v}

_{c}###

*c*

*c*

*v*

*l*

*s*

*l*

*E*

*e*

*E*

*w*

*h*

*N*

*E*

_{} tan tan (11b) 501 502

*Equations (9)-(11) lead to a quadratic polynomial of tan2 θ: *
503

###

*n*

_{sc}**

_{l}*K*

###

tan4*e*tan2

_{v}###

*n*

_{sc}*1*

_{l}###

0 (12a) 504Equation (12a) can be rewritten in a simple form as
505
tan4 tan2 0
*C*
*B*
*A* (12b)
506
where
507

###

###

*n*

_{sc}**

_{l}*A*,

*B e*and

_{v}*C*

###

*n*

_{sc}*1*

_{l}###

(12c) 508###

_{t}

_{Ft}

_{Fs}###

*F*

*Ft*

*s*

*t*

*t*

*s*

*l*

*n*

*E*

*E*

*E*

_{}

_{} (12d) 509

*c*
*s*
*sc*
*E*
*E*
*n* ;
*s*
*F*
*Fs*
*E*
*E*
*n* ;
*c*
*c*
*c*
*v*
*v*
*E*
*w*
*h*
*N*
*e * ; * _{t}*

**

_{t}**

_{Ft}n_{fs}**

_{t}**

_{Ft}n_{fs}_{0}

*(12e) 510 511*

_{t}*Step (b) After the yielding of the transverse reinforcement but before the yielding of the *

512

*longitudinal reinforcement *

513

*The analysis is conducted in a similar manner to that described in Step (a), but in this case ft*

514

*is replaced by the yield strength of the transverse reinforcement (fyt). By substituting Esεt* by

515

*fyt into Equations (9)-(11), the polynomial of tan θ can be written as: *

516
1 tan4 1 tan2 1 1_{}0
*l*
*sc*
*v*
*l*
*sc*
*t*
*sc* *n*
*e*
*n*
*n* (13)
517
where _{Ft}_{fs}_{t}_{Ft}_{fs}_{t}*s*
*yt*
*t* *n* *n*
*E*
*f*
*H* _{0} (14)
518
519

*Step (c) After the yielding of both the transverse and longitudinal reinforcement *

520

*The analysis is conducted in a similar manner to that described in Step (a), but in this case ft*

521

*is replaced by fyt and fl is replaced by the yield strength of the longitudinal reinforcement (fyl*).

522

*By substituting Esεt by fyt and Esεl by fyl, into Equations (9)-(11), the polynomial of tan θ can *

523
be written as:
524
1 tan4 1 tan2 0
*H*
*E*
*f*
*n*
*n*
*H*
*s*
*yl*
*sc*
*t*
*sc*
(15)
525

*where H is given by Equation (14). *
526

527 528

*Step (d) After the yielding of the longitudinal reinforcement but before the yielding of the *

529

*transverse reinforcement *

*The analysis is conducted in a similar manner to that described in Step (a), but in this case fl*

531

*is replaced by fyl. By substituting Esεl by fyl into Equations (9)-(11), the polynomial of tan θ *

532

can be written as:
533
tan4 1 _{}tan2 0
*T*
*E*
*f*
*n*
*E*
*E*
*n*
*E*
*E*
*s*
*yl*
*sc*
*F*
*Ft*
*s*
*t*
*t*
*Fs*
*Ft*
*c*
*t*
*t*
*c*
(16)
534
where *t**t* *FtnFs**t* *FtnFs*0*t* (17)
535
536
*Solution procedure *
537

Initial inputs are required to calculate the stresses and strains in the joint up to failure. The 538

inputs can be categorized into: (a) geometric variables (beam and column cross-sections, 539

effective width and depth of the joint, horizontal (beam) and vertical (column) reinforcement 540

*ratios, and existing and embedded joint reinforcement ratios); (b) bond condition variables (βt*

541

*and βl*); (c) material properties (concrete strength; concrete stress-strain properties (see

542

Equation 18); elastic moduli of the concrete, steel and FRP; yield strengths of the beam, 543

column and joint reinforcement; and debonding properties of the embedded bars (see 544

*Equation 19) ); (d) the axial force acting on the column and (e) the initial normal strain ε0t*.

545 546

*The procedure is initiated by incrementing the transverse strain, εt*. Prior to first yielding of

547

*the steel reinforcement, Equation (12b) is solved for tan θ and the shear stress in the joint *
548

area is calculated using Equation (11a). At each step of the calculation, the stresses in both 549

the transverse (beam and joint) and longitudinal (column) reinforcement are checked against 550

their yield strengths. Post yielding of the steel reinforcement, Equations (13), (15) or (16) are 551

activated depending on the yield sequence of the longitudinal and transverse reinforcement. 552

*The value of tan θ is obtained by solving the equation corresponding to the active scenario in *
553

each step. Next, the normal stress in the embedded bars, along the transverse direction at the 554

mid-height of the joint, is evaluated. At the end of each step, two failure modes are checked: 555

concrete crushing and debonding of the embedded bars. 556

557

*Concrete crushing occurs when σ2 reaches the maximum concrete strength (fc* *max*) as defined

558

in Equation (18) (Pantazopoulou and Bonacci, 1992).
559
560
2
max
2
max
2
max
2 2 _{}
*fc* (18.a)
561

###

###

0 1 0 max max 34 . 0 8 . 0 1 *c*

*ys*

*sv*

*c*

*c*

*f*

*f*

*f*

*f*(18.b) 562

*where ε0 is the failure strain of concrete in uniaxial compression (taken as -0.002), ρsv* is the

563

*volume ratio of stirrups and fys* is the yield stress of stirrups.

564 565

On the other hand, debonding of the embedded bars takes place when the maximum bond 566

*strength between the concrete and the embedded bars (τb,max*) is exceeded. For embedded

567

*CFRP bars, τb,max* is defined by Equation (19a) (Okelo and Yuan, 2005); whereas for

568

*embedded steel bars, τb,max* is defined by Equation (19b) (CEB-FIP, 1993).

569
*b*
*c*
*b*
*d*
*f*
7
.
14
max
,
(19a)
570
_{b}_{,}_{max} 2.0

###

*f*8

_{c}###

(19b) 571 572*Comparison between predicted and experimental results *

573

The analytical model was used to predict the shear strength of the tested RC BCJs. Table 5 574

compares the predicted and experimental results. Perfect bond was assumed between the 575

*concrete and the longitudinal and transverse reinforcement, corresponding to βt = βl* = 0. It is

576

evident from Table 5 that the proposed model gives excellent results in terms of both 577

accuracy and precision. The model had an overall average predicted-to-experimental ratio of 578

1.05 with a standard deviation of 0.04. The strengthened RC BCJs had predicted-to-579

experimental ratios ranging from 1.02 to 1.07 whereas the control specimens had predicted-580

to-experimental ratios ranging from 1.01 to 1.11. This result suggests that the shear strength 581

of the strengthened specimens is better predicted by the model. It is recommended that 582

additional tests be carried out to further evaluate the accuracy of the proposed model and 583

expand the database of RC BCJs strengthened with embedded bars. 584

585

**Conclusions **
586

This study presents results of an experimental and analytical investigation on the structural 587

performance of exterior RC BCJs strengthened with embedded bars. It also provides insight 588

into the effect of type (CFRP or steel) and number (four or eight) of embedded bars on the 589

structural behavior of the strengthened BCJs. Based on the results of this study, the following 590

conclusions are drawn. 591

All strengthened specimens experienced less damage and had an improved load and/or 592

deformation capacity compared with the control specimen. 593

Due to the lower elastic modulus of the CFRP bars compared with that of the steel bars, 594

the embedded CFRP bars had higher strain than the corresponding steel bars. For both 595

embedded bar types, increasing the number of bars from 4 to 8 bars reduced the strain in 596

the embedded bars. 597

The strengthened specimens exhibited enhancements in joint shear strength and 598

normalized principal tensile stress at peak load of 6-21% and 18-25%, respectively, 599

compared with the control specimen. The strengthened specimens also outperformed the 600

adequately designed specimen. 601

The strengthened specimens were 6-93% more ductile compared with the control 602

specimen. Due to the ductile nature of the steel bars, the steel-strengthened specimens 603

exhibited a more ductile behavior than the CFRP-strengthened specimens did. 604

The energy dissipation capacity and peak-to-peak stiffness of the strengthened specimens 605

were 10-54% and 2-35%, respectively, higher than those of the control specimen. Both 606

parameters increased with the increase in the number of embedded bars. The results 607

suggest that the type of embedded bar has insignificant effect on energy dissipation 608

capacity and peak-to-peak stiffness. 609

The control specimen had limited beam fixed-end rotation, indicating the absence of a 610

plastic hinge in the beam. On the other hand, the strengthened specimens had much 611

higher beam fixed-end rotation, suggesting the onset of a beam hinge mechanism. 612

Moreover, the steel-strengthened specimens had higher beam fixed-end rotation 613

compared with the CFRP-strengthened specimens. 614

A design model is developed for RC BCJs strengthened with embedded bars. The 615

accuracy of the proposed model is verified against the experimental results reported in 616

this study. The proposed model showed good correlation with the experimental results, 617

attaining an average predicted-to-experimental ratio and a standard deviation of 1.05 and 618

0.04, respectively. 619

**Acknowledgements **
621

The first author highly appreciates the financial support provided by the Directorate General 622

of Higher Education, Ministry of Research and Higher Education of Indonesia through Grant 623

323/E4.4/K/2012. The authors gratefully acknowledge the support provided by the technical 624

staff of the Structures Laboratory at the University of Birmingham. 625

626

**References **
627

*ACI 352R-02. (2002). Recommendations for Design of Beam-Column Connections in *
628

*Monolithic Reinforced Concrete Structures, American Concrete Institute, Farmington *

629

Hills, Mich. 630

*ACI T1.1-01. (2001). Acceptance Criteria for Moment Frames Based on Structural Testing, *
631

American Concrete Institute, Farmington Hills, Mich. 632

Akguzel, U., and Pampanin, S. (2012). "Assessment and Design Procedure for the Seismic 633

Retrofit of Reinforced Concrete Beam-Column Joints using FRP Composite 634

*Materials." ASCE Journal of Composites for Construction, 16(1), 21-34. *
635

Antonopoulos, C. P., and Triantafillou, T. C. (2002). "Analysis of FRP-Strengthened RC 636

*Beam-Column Joints." ASCE Journal of Composites for Construction, 6(1), 41-51. *
637

Antonopoulos, C. P., and Triantafillou, T. C. (2003). "Experimental Investigation of FRP-638

*Strengthened RC Beam-Column Joints." ASCE Journal of Composites for *
639

*Construction, 7(1), 39-49. *

640

Bedirhanoglu, I., Ilki, A., Pujol, S., and Kumbasar, N. (2010). "Behavior of Deficient Joints 641

*with Plain Bars and Low-Strength Concrete." ACI Structural Journal, 107(3), *
300-642

310. 643

*CEB-FIP. (1993). CEB-FIP Model Code 1990, Comite Euro-International du Beton, *
644

Lausanne, Switzerland. 645

Chaallal, O., Mofidi, A., Benmokrane, B., and Neale, K. (2011). "Embedded Through-646

Section FRP Rod Method for Shear Strengthening of RC Beams: Performance and 647

*Comparison with Existing Techniques." ASCE Journal of Composites for *
648

*Construction, 15(3), 374-383. *

649

Dirar, S., Lees, J. M., and Morley, C. T. (2013). "Precracked Reinforced Concrete T-beams 650

*Repaired in Shear with Prestressed Carbon Fibre-Reinforced Polymer Straps." ACI *
651

*Structural Journal, 110(5), 855-866. *

652

Dolce, M., and Goretti, A. (2015). "Building Damage Assessment After The 2009 Abruzzi 653

*Earthquake." Bulletin of Earthquake Engineering, 13, 2241-2264. *
654

El-Amoury, T., and Ghobarah, A. (2002). "Seismic Rehabilitation of Beam-Column Joint 655

*using GFRP Sheets." Engineering Structures, 24(11), 1397-1407. *
656

Engindeniz, M., Kahn, L. F., and Zureick, A. (2005). "Repair and Strengthening of 657

*Reinforced Concrete Beam-Column Joints: State of the Art." ACI Structural Journal, *
658

102(2), 187-197. 659

Garcia, R., Jemaa, Y., Helal, Y., and Guadagnini, M. (2014). "Seismic Strengthening of 660

*Severely Damaged Beam-Column RC Joints Using CFRP." ASCE Journal of *
661

*Composites for Construction, 18(2), 04013048. *

662

Ghobarah, A., and El-Amoury, T. (2005). "Seismic Rehabilitation of Deficient Exterior 663

*Concrete Frame Joints." ASCE Journal of Composites for Construction, 9(5), *
408-664

416. 665

Ghobarah, A., and Said, A. (2002). "Shear Strengthening of Beam-Column Joints." 666

*Engineering Structures, 24(7), 881-888. *

667

González, A. D., Dueñas-Osorio, L., Sánchez-Silva, M., and Medaglia, A. L. (2016). "The 668

Interdependent Network Design Problem for Optimal Infrastructure System 669

*Restoration." Computer-Aided Civil and Infrastructure Engineering, 31(5), 334-350. *
670

Karayannis, C. G., Chalioris, C. E., and Sirkelis, G. M. (2008). "Local Retrofit of Exterior 671

RC Beam–Column Joints using Thin RC Jackets—An Experimental Study." 672

*Earthquake Engineering & Structural Dynamics, 37(5), 727-746. *

673

Li, C. Y., and Mobasher, B. (1998). "Finite Element Simulations of Fiber Pullout Toughening 674

*in Fiber Reinforced Cement Based Composites." Advanced Cement Based Materials, *
675

7(3–4), 123--132. 676

Okelo, R., and Yuan, R. L. (2005). "Bond Strength of Fiber Reinforced Polymer Rebars in 677

*Normal Strength Concrete." ASCE Journal of Composites for Construction, 9(3), *
203-678

213. 679

Pampanin, S., Christopoulos, C., and Chen, T. H. (2006). "Development and Validation of a 680

Metallic Haunch Seismic Retrofit Solution for Existing Under-designed RC Frame 681

*Buildings." Earthquake Engineering & Structural Dynamics, 35(14), 1739-1766. *
682

Pantazopoulou, S., and Bonacci, J. (1992). "Consideration of Questions about Beam-Column 683

*Joints." ACI Structural Journal, 89(1), 27-36. *
684

Pantelides, C. P., Clyde, C., and Reaveley, L. D. (2002). "Performance-Based Evaluation of 685

*Reinforced Concrete Building Exterior Joints for Seismic Excitation." Earthquake *
686

*Spectra, 18(3), 449-480. *

687

Park, R. (1989). "Evaluation of Ductility of Structures and Structural Assemblages from 688

*Laboratory Testing." Bulletin of the New Zealand National Society for Earthquake *
689

*Engineering, 22(3), 155-166. *

690

Park, Y. J., and Ang, A. H. S. (1985). "Mechanistic Seismic Damage Model for Reinforced 691

*Concrete." ASCE Journal of Structural Engineering, 111(4), 722-739. *
692

Park, Y. J., Ang, A. H. S., and Wen, Y. K. (1987). "Damage-Limiting Aseismic Design of 693

*Buildings." Earthquake Spectra, 3(1), 1-26. *
694

Qapo, M., Dirar, S., and Jemaa, Y. (2016). "Finite Element Parametric Study of Reinforced 695

*Concrete Beams Shear-Strengthened with Embedded FRP Bars." Composite *
696

*Structures, 149, 93-105. *

697

Qin, S., Dirar, S., Yang, J., Chan, A. H. C., and Elshafie, M. (2015). "CFRP Shear 698

*Strengthening of Reinforced-Concrete T-Beams with Corroded Shear Links." ASCE *
699

*Journal of Composites for Construction, 19(5), 04014081. *

700

Sasmal, S., and Nath, D. (2017). "Seismic Performance of Non-invasive Single Brace Made 701

of Steel and Shape Memory Alloy for Retrofit of Gravity Load Designed Sub-702

*assemblages." Engineering Structures, 143, 316-329. *
703

Tsonos, A. G. (2008). "Effectiveness of CFRP-Jackets and RC-Jackets in Post-earthquake 704

*and Pre-earthquake Retrofitting of Beam-Column Subassemblages." Engineering *
705

*Structures, 30, 777-793. *

706

Valerio, P., Ibell, T. J., and Darby, A. P. (2009). "Deep embedment of FRP for concrete shear 707

*strengthening." Structures and Buildings, 162(5), 311-321. *
708

Varum, H. (2003). "Seismic Assessment, Strengthening and Repair of Existing Buildings." 709

PhD thesis, University of Aveiro, Aveiro, Portugal. 710

Yurdakul, Ö., Tunaboyu, O., and Avşar, Ö. (2018). "Retrofit of Non-seismically Designed 711

Beam-Column Joints by Post-tensioned Superelastic Shape Memory Alloy Bars." 712

*Bulletin of Earthquake Engineering, in press. *

713 714 715 716 717 718 719

**List of Figures **
720

721

Fig. 1. Reinforcement details of the test specimens, unit in mm. 722

Fig. 2. Strengthening configuration. 723

Fig. 3. Schematic drawing of the experimental set-up. 724

Fig. 4. Loading history. 725

Fig. 5. Load versus displacement curves. 726

Fig. 6. Crack patterns of the tested specimens at peak load (corresponding to 3.00% drift 727

ratio). 728

Fig. 7. Damage versus drift ratio. 729

Fig. 8. Envelope curves of load versus strain in the embedded bars. 730

Fig. 9 Envelope curves of normalized principal tensile stress versus joint shear deformation 731

Fig. 10. Comparison of energy dissipation. 732

Fig. 11. Comparison of normalized peak-to-peak stiffness. 733

Fig.12. Envelope curves of normalized load versus beam fixed-end rotation. 734

Fig. 13. Idealization of an external beam-column joint, based on Akguzel and Pampanin 735

(2012): (a) Moments and shear forces acting on the boundaries of the plane frame element; 736

(b) Kinematics and compatibility conditions in joint region; (c) Mohr’s circle for average 737

stresses. 738

Fig. 14. Stress equilibrium in a joint with embedded bars, modified after Antonopoulos and 739 Triantafillou (2002). 740 741 742 743

744

745

**Fig. 1. Reinforcement details of the test specimens, unit in mm. **
746

747 748 749 750

**Fig. 2. Strengthening configuration. **
751

752

753

a) Acrylic rods within specimens with four embedded bars 754 755 756 757 758 759 760 761 762 763

764 765

b) Acrylic rods within specimens with eight embedded bars 766 767 768 769 770 771 772 773 774 775 776

777 c) Cast-in-concrete holes 778 779 780 781 782 783 784 785 786 787 788 789

790 791

d) Application of embedded bars 792 793 794 795 796 797 798 799 800 801 802

803

**Fig. 3. Schematic drawing of the experimental set-up. **
804

805 806 807 808

809

**Fig. 4. Loading history. **
810
811
812
813
814
815
816
817
818
819
820
821
822
823
824

**Fig. 5. Load versus displacement curves. **
825
826
(a) BCJ-CS-A
827
828
829
830
831
832
833

834 (b) BCJ-SS-S4 835 836 837 838 839 840 841 842

843 (c) BCJ-SS-F4 844 845 846 847 848 849 850 851

852 (d) BCJ-SS-S8 853 854 855 856 857 858 859 860

861 (e) BCJ-SS-F8 862 863 864 865 866 867 868 869

870 (f) BCJ-CS-B 871 872 873 874 875 876 877 878

879

(g) Envelope curves for tested specimens 880 881 882 883 884 885 886 887

**Fig. 6. Crack patterns of the tested specimens at peak load (corresponding to 3.00% drift **
888
ratio).
889
890
(a) BCJ-CS-A
891
892
893
894
895
896
897
898
899
900

901 (b) BCJ-SS-S4 902 903 904 905 906 907 908 909 910 911

912 (c) BCJ-SS-F4 913 914 915 916 917 918 919 920 921 922 923

924 (d) BCJ-SS-S8 925 926 927 928 929 930 931 932 933 934 935

936 (e) BCJ-SS-F8 937 938 939 940 941 942 943 944 945 946 947

948 (f) BCJ-CS-B 949 950 951 952 953 954 955 956 957 958 959 960

961

**Fig. 7. Damage versus drift ratio. **
962
963
964
965
966
967
968
969
970
971
972
973
974
975

976

**Fig. 8. Envelope curves of load versus strain in the embedded bars. **
977
978
979
980
981
982
983
984

985

**Fig. 9. Envelope curves of normalized principal tensile stress versus joint shear deformation. **
986
987
988
989
990
991
992

993 994

**Fig. 10. Comparison of energy dissipation. **
995
996
997
998
999
1000
1001
1002
1003

1004

**Fig. 11. Comparison of normalized peak-to-peak stiffness. **
1005
1006
1007
1008
1009
1010
1011
1012

1013

**Fig.12. Envelope curves of normalized load versus beam fixed-end rotation. **
1014
1015
1016
1017
1018
1019
1020

**Fig. 13. Idealization of an external beam-column joint, based on Akguzel and Pampanin **
1021
(2012).
1022
1023
1024

(a) Moments and shear forces acting on the boundaries of the plane frame element; 1025 1026 1027 1028 1029 1030

1031

**(b) Kinematics and compatibility conditions in joint region **
1032
1033
1034
1035
1036
1037
1038
1039
1040
1041
1042
1043

1044 1045

(c) Mohr’s circle for average stresses. 1046 1047 1048 1049 1050 1051 1052 1053 1054 1055 1056 1057 1058 1059

**Fig. 14. Stress equilibrium in a joint with embedded bars, modified after Antonopoulos and **
1060

Triantafillou (2002). 1061

1062

(a) Horizontal forces 1063 1064 1065 1066 1067 1068 1069 1070 1071 1072

1073
1074
**(b) Vertical forces **
1075
1076
1077
1078
1079
1080
1081
1082
1083
1084
1085

**List of Tables **
1086

1087

Table 1. Details of the tested beam-column joint specimens. 1088

Table 2. Concrete properties. 1089

Table 3. Steel reinforcement properties. 1090

Table 4. Summary of test results. 1091

Table 5. Comparison between experimental and predicted results. 1092 1093 1094 1095 1096 1097 1098 1099 1100 1101 1102 1103 1104 1105 1106 1107 1108 1109 1110